Relationship between the Thermally Induced Reorientations of Aromatic Solvate Molecules in Cu(hfac)2- Nitroxide Breathing Crystals and the Character of the Magnetic Anomaly
Galina V. Romanenko; Ksenia Yu. Maryunina; Artem S. Bogomyakov; Renad Z. Sagdeev; Victor I. Ovcharenko; Inorganic Chemistry 50 (2011) 6597–6609; doi:10.1021/ic200444e

data_4325655
_publ_section_title
;
 Relationship between the Thermally Induced Reorientations of Aromatic
 Solvate Molecules in Cu(hfac)2- Nitroxide Breathing Crystals and the
 Character of the Magnetic Anomaly
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6597
_journal_page_last               6609
_journal_paper_doi               10.1021/ic200444e
_journal_volume                  50
_journal_year                    2011
_chemical_formula_sum            'C28 H27 Cu F15 N4 O6'
_chemical_formula_weight         864.08
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                98.223(6)
_cell_angle_beta                 97.348(6)
_cell_angle_gamma                111.840(6)
_cell_formula_units_Z            2
_cell_length_a                   11.0848(11)
_cell_length_b                   13.4222(13)
_cell_length_c                   13.4220(13)
_cell_measurement_temperature    240
_cell_volume                     1798.6(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      240
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.987
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0509
_diffrn_reflns_av_sigmaI/netI    0.0761
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            22271
_diffrn_reflns_theta_full        27.98
_diffrn_reflns_theta_max         27.98
_diffrn_reflns_theta_min         2.02
_exptl_absorpt_coefficient_mu    0.730
_exptl_absorpt_correction_T_max  0.9306
_exptl_absorpt_correction_T_min  0.7491
_exptl_crystal_colour            dark
_exptl_crystal_density_diffrn    1.596
_exptl_crystal_description       bulk
_exptl_crystal_F_000             870
_exptl_crystal_size_max          0.42
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.462
_refine_diff_density_min         -0.350
_refine_diff_density_rms         0.049
_refine_ls_extinction_coef       0.0042(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.863
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     662
_refine_ls_number_reflns         8561
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      0.886
_refine_ls_R_factor_all          0.0873
_refine_ls_R_factor_gt           0.0432
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0515P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0982
_refine_ls_wR_factor_ref         0.1114
_reflns_number_gt                4606
_reflns_number_total             8561
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic200444e_si_002_60.cif
_cod_data_source_block           f3f3240
_cod_database_code               4325655